extensional flow characterisation and extrusion blow ... and extrusion blow moulding of ... haworth...
Post on 06-Mar-2018
Embed Size (px)
Loughborough UniversityInstitutional Repository
Extensional flowcharacterisation and
extrusion blow moulding ofhigh density polyethylene
modified by calciumcarbonate
This item was submitted to Loughborough University's Institutional Repositoryby the/an author.
Citation: HAWORTH, B. and JUMPA, S., 1999. Extensional flow character-isation and extrusion blow moulding of high density polyethylene modified bycalcium carbonate. Plastics, Rubber and Composites, 28 (8), pp. 363-378
This article was published in the journal, Plastics, Rubberand Composites [ c Maney Publishing] and is available at:http://www.maney.co.uk/search?fwaction=show&fwid=199
Metadata Record: https://dspace.lboro.ac.uk/2134/4228
Publisher: c Maney
Please cite the published version.
This item was submitted to Loughboroughs Institutional Repository (https://dspace.lboro.ac.uk/) by the author and is made available under the
following Creative Commons Licence conditions.
For the full text of this licence, please go to: http://creativecommons.org/licenses/by-nc-nd/2.5/
Extensional flow characterisation and extrusionblow moulding of high density polyethylene
modified by calcium carbonateB. Haworth and S. Jumpa
Free surface elongational flow properties, including transient state stressgrowth and melt rupture data, have been measured on a range of calciumcarbonate filled high density polyethylene (HDPE) compounds, using aRutherford elongational rheometer operating at constant strain rate inthe range 0160 s1. Results show that polymer molecular weight has astrong influence on both tensile stress growth and melt rupture data; in-creasing elongational strain rate decreases the stress growth coefficient,in all compounds. At any specific elongational strain rate, the stress growthcoefficient increases with volume fraction of particulate additives and alsowhen using additives of fine particle size, as a result of packing fraction effects.Acid coatings added at super-monolayer levels influence the viscosity of highlyfilled compounds, by internal lubrication.
Dynamic extrusion data obtained by experimental blow moulding of calciumcarbonate modified HDPE materials show that modifications to melt stateshear modulus result in reduced die swell, to an extent determined by fillercoating. In combination with die swell, higher extensional viscosity of filledHDPE contributes significantly to enhanced parison sag resistance. Solid statemodulus enhancement was consistently observed in calcium carbonate filledHDPE containers and if excellent filler dispersion can be achieved, it is feasibleto retain the ductile mode failure of unfilled HDPE when containers aresubjected to high velocity impact loads. PRC/1576
1999 IoM Communications Ltd. At the time the work was carried outthe authors were at the Institute of Polymer Technology and MaterialsEngineering, Loughborough University, Loughborough, Leicestershire LE113TU, UK. Dr Jumpa is now in the Department of Chemistry, King Mong-kuts Institute of Science and Technology Ladkrabang, Chalongkrung Road,Ladkrabang, Bangkok 10520, Thailand. This paper was presented at Advancesin Blow Moulding held in Loughborough, UK on 30 June1 July 1998.
INTRODUCTION AND BACKGROUND (ii) the interfacial adhesion characteristics betweenMineral fillers can be loosely classified as inactive the particles and the resin matrix, which influ-(extenders, or cost reducing additives) or as active ence the ultimate mechanical properties of the(functional ) additives, which induce specific changes composite materials.in properties so that the compound largely meets the Incorporation of particulate additives into a resinrequirements demanded of it.1 Currently, there is leads to modified processing behaviour and occasion-renewed interest in the use of mineral fillers to achieve ally to a subsequent deterioration of the ultimateenhanced processing of thermoplastics, particularly if mechanical performance.7 However, some importantin addition, some specific physical properties of the aspects of mechanical behaviour can be significantlyproduct can also be improved. Fillers can change the enhanced by filler addition; for example, enhancedcharacteristics of a polymer in two ways: the prop- melt fracture stress occurs when processing fillederties of the particles (size, shape, modulus, and surface elastomers.8 Toughness enhancement has also beenenergy) can have profound effects on melt state and noted in polyalkenes and in brittle matrix polymers,9solid phase mechanical behaviour and also a change
as long as certain criteria are fulfilled. For example,in the micromorphology of the solidified polymer
a critical factor that influences mechanical propertiesmay occur, giving rise to differences in the observed
of the compound is the state of particle dispersion insolid state properties. For example, increases inthe matrix.10,11 To facilitate filler dispersion, the filleraddition level of fillers (such as CaCO3 and carbon is often surface treated with a coating, which acts asblack, (CB)) in polyalkenic compounds generallya wetting agent by reducing the specific surface freeimproves low strain properties such as tensile modu-energy of the additive particles. Common coatinglus,25 but may decrease properties relating to energyagents for mineral fillers are fatty acids, from whichabsorption, such as ultimate tensile strength2,6 andthe acid group reacts onto the filler surface. However,elongation at break.3,5the hydrocarbon chain is unable to react chemicallyAdditionally, two important technical issues mustwith the matrix and interacts only weakly, producingbe considered when using fillers:low bond strength between filler and matrix.12 The(i) the rheological behaviour of the filled polymereffect is therefore one of reduced physical interaction,(melt state mechanical behaviour), whichrather than a direct, adhesion promoting phenom-governs processability and influences micro-
structure development enon. In summary, treatment of CaCO3 with stearic
Plastics, Rubber and Composites 1999 Vol. 28 No. 8 363ISSN 14658011
364 Haworth and Jumpa Extensional flow characterisation and extrusion blow moulding of CaCO3
acid decreases the surface energy of the filler and oped by Smoker26 who studied the elongational flowbehaviour of low density polyethylene (LDPE) forparticleparticle interactions within agglomerated
regions. This facilitates filler dispersion and also film blowing applications. Further modifications ofthe RER apparatus were subsequently introduced byleads to enhanced mechanical performance of the
compounds.13,14 Previous research15 using coatings Axtell and Haworth27,28 who used the RER to studythe viscoelastic behaviour of poly(ethylene terephthal-of different aliphatic chain length in filled polyethylene
has demonstrated that when longer chain coating ate) (PET) in the rubbery region at temperaturesabove the primary glass transition temperature Tg , toagents are used to treat the fillers, low strain modulus
and yield stress are enhanced but compounds are simulate the stretchblow moulding process. Otherapplications have been focused upon rigid PVC com-more prone to brittle mode failure as a result of lower
energy absorption. pounds, to simulate elongational deformation andflow in processes such as thermoforming, and bubbleImprovements in process equipment have been
made to enhance efficiency in the compounding of formation in foam extrusion.29 Very little previousresearch has been reported relating to the elongationalfillers and other particulate additives16 and a study
of the rheological characteristics of newly formulated deformation and rupture of filled polymer melts. Ithas been reported30 that in fibre filled polypropylenecompounds is a most important step in examining
their behaviour in polymer conversion processes such compounds, the elongational viscosity is not only afunction of time but also of strain rate. Other work-as extrusion blow moulding. The viscoelastic flow
behaviour of particle filled polymer melts depends ers21 have reported that the elongational viscosity ofCaCO3 filled polystyrene increases with filler contentupon the filler characteristics, the nature of the (poly-
mer/particle and particle/particle) interfaces, the and/or reduction of particle size.This research focuses on composite systems of highdegree of dispersion, and the orientation distribution
of the filler particles.17 The presence of other additives, molecular weight, high density polyethylene (HDPE)resins compounded with a number of CaCO3 fillerseven in small quantities, may be crucial in the compos-
ite system because they may interfere with the resin/ varying in particle size, surface coating, and additionlevel. The filler coatings include stearic acid, which isfiller interface18 and may also influence the intera-
ction between the compound and machinery surfaces a widely used coating agent in filled polyalkeniccompounds, and an acid terminated polyethyleneto create a wall slip effect at the flow boundary.19
Generally, the presence of filler particles increases the (ATPE), a newly developed material based upon lowmolar mass polyethylene chains terminated at onepolymer melt viscosity,20 with highest levels of vis-
cosity being observed at higher filler content3,5 or end with an acid group.